Chapter 4 The Properties of Electroless Nickel Rolf Weil and Konrad Parker Electroless nickel deposits are used by many industries as functional coatings because they possess a unique combination of both corrosion and wear resistance. The ability to coat parts, regardless of their size, with a deposit of uniform thickness is another desirable property of electroless nickel. As is the case for electrodeposits, most of the properties of electroless nickel are structure-dependent. However, as its structure and composition are quite different from those of electrodeposited nickel, its properties differ also. The structures and properties of two groups of electroless nickel (EN) deposits will be considered in this chapter. In the first group are nickelphosphorus alloys, which are deposited from solutions in which sodium hypophosphite is the reducing agent. These deposits typically have phosphorus contents of 7 to 11 percent (all compositions in this chapter are in weight percent). Nickel-boron alloys constitute the second group. They are obtained from solutions in which either an organic aminoborane or sodium borohydride is the reducing agent. Typical boron contents of such deposits are 0.2 to 4 percent or 4 to 7 percent, respectively. The deposit plated in sodium borohydride solutions usually also contain 4 to 5 percent thallium. EN deposits containing particles of materials such as silicon carbide, diamonds, alumina, and PTFE are discussed elsewhere in this book. STRUCTURE OF ELECTROLESS NICKEL As-deposited electroless nickel is a metastable, supersaturated alloy. The equilibrium phase diagrams (1) of the Ni-P and Ni-B systems shown in Figs. 4.1 and 4.2 exhibit essentially no solid solubility of phosphorus or boron in nickel at ambient temperatures. Under equilibrium conditions, therefore, the alloys consist of essentially pure nickel and the intermetallic compound Ni3Por Ni3B. The conditions existing during plating, however, do not permit the formation of the intermetallic compounds. Even the growth of very tiny crystals would involve the movement of large numbers of atoms by surface diffusion in order to achieve the correct stoichiometry of three nickel atoms to one phosphorus or boron atom. This movement cannot occur before the next layer of atoms has been laid down; thus, the phosphorus or boron atoms are trapped between nickel atoms, resulting in supersaturation. There is experimental evidence (2,3)that 111 112 ELECTROLESS PLATING Fig. 4.1-Nickel-phosphorus phase diagram (1). phosphorus atoms so trapped are not uniformly distributed. There are very small regions where one-third of the atoms are phosphorus, and others where there is essentially pure nickel. The crystal structure of nickel is face-centered-cubic (fcc), in which each atom has 12 near neighbors. The entrapment of phosphorus or boron makes it impossible for this atom arrangement to extend over large surfaces. The volume of material within which the fcc atom arrangement can be maintained is called a grain. Grain sizes are very small in electroless nickel. If the fcc structure cannot be maintained at all, the structure is equivalent to that of a liquid and is considered to be amorphous. Low-alloy electroless nickel deposits are microcrystalline, that is, they consist of many very small grains. Values of about 2 and 6 nm (1 nm = 10 angstroms), as determined from the broadening of diffraction peaks, have been reported (4) for Ni-B and Ni-P, respectively. Other investigators (5),have also reported a grain size of about 2 nm for Ni-P. Phosphorus contents of <7 percent result in microcrystalline deposits (6). Deposits having higher alloy contents can be considered amorphous, with their diffraction patterns consisting of only one broad peak or ring. An electron diffraction pattern showing one such broad ring is illustrated in Fig. 4.3. The Properties of Electroless Nickel 113 Fig. 4.2-Nickel-boron phase diagram (1). Careful analysis (7) of X-ray diffraction patterns of electrodeposits containing 12 to 13 percent P has shown, however, that even high-alloy deposits.may contain small regions that are microcrystalline. Nevertheless, since the diffraction patterns of the high-alloy electroless nickel deposits are very similar to those of materials that are rapidly cooled from the liquid state (6) and that are considered to be glasses, electroless nickel can justifiably be considered amorphous. A typical structure of a high-phosphoruselectroless nickel deposit, as seen in a thin foil by transmission electron microscopy (TEM), isshown in Fig. 4.3. No grains or other prominent structural features are seen. The structure, as seen by optical microscopy, of metallographically polished and properly etched cross sections of electroless nickel show the so-called banded or lamellar structure depicted in Fig. 4.4. This structure has been attributed to compositional variations with deposit thickness (8,9). The cause of the compositional variation has been explained (10) in terms of periodic fluctuations in the pH of the plating solution adjacent to the deposit surface. These fluctuations, which result in variations of the phosphorus content, were postulated as being caused by hydrogen evolution, which raised the pH. The resulting stirring action then lowered the pH by mixing the plating solution adjacent to the deposit with the bulk of the bath. Markings perpendicular to the 114 ELECTROLESS PLATING Fig. 4.3-TEM photo of a high-phosphorus electroless nlckel deposit. inset shows electron diffraction pattern. Flg. 4.4-Optical micrograph of metallographically pollrhed and etched cross-section of an amorphous, unannealed electroless nickel deposit. Banded structure Is evldent. The Properties of Electroless Nickel 115 banded structure can also be seen in Fig. 4.4. Sometimes these markings can appear similar to those of a columnar structure. However, as the grain size is much too small to be resolved with an optical microscope, the structure is not the columnar one exhibited by electrodeposits. The structural changes that occur when amorphous electroless nickel deposits are annealed above 300" Care illustrated in Figs. 4.5 and 4.6. First, the amorphous structure crystallizes, as seen in Fig. 4.5. This structural change is accompanied by the evolution of the heat of crystallization. Figure 4.6 shows the completion of crystallization. The grains have become somewhat larger but are still very small. Intermediate processes during the formation of intermetallic compounds can result in precipitation or age hardening. Particles of a precipitate form when sufficient atoms diffuse to a particular location to form a volumeof material that has the correct stoichiometric composition and that is large enough so that a boundary can form around it. Before the volume of material reaches this critical size, its atom arrangement and that of the surrounding matrix must remain continuous. This coherency between regions having different interatomic spacings results in severestraining, which hardens thealloy. The initial stageof the precipitation of the intermetallic phase, which is still coherent with the matrix, can be seen in Fig. 4.6. The small dark particles are the coherent precipitate. Fig. 4.5-TEM photo 01 originallyamorphous NI-P deposit annealed at 310" C, resultlng In crystallization. Flg. 4.6-TEM of orlglnally amorphous NI-P deposit annealed at 375" C. Crystalllzatlonis complete and a coherent precipitate Is evldent. 116 ELECTROLESS PLATING Graphs of hardness vs. aging time at several temperatures for an electroless Ni-P alloy (11) are shown in Fig. 4.7. These graphs are very similar to those of age-hardenable aluminum alloys. Above 450" C the times are too short to be practical for age hardening. An aging temperature of 400" C appears to be the most practical for deposits on steel, as only a short time is needed. A hardness of 900 to 1000 HV can also be attained by heating at lower temperatures for longer periods, e.g., >260" C for more than 6 hr. Age-hardening curves for Ni-B alloys (13) are shown in Fig. 4.8. Again, it is seen that in a relatively short annealing time, the maximum hardness can be attained at 400" C. Deposit overaging occurs when hardness values peak and then decline with increasing heat treatment, due to the formation of NilP crystals, as shown in Fig. 4.9. The increase in the sizes of grains of the nickel matrix and the Ni,P phase further reduces the hardness, as does diffusion of phosphorus to the surface. Ni-B alloys tend to maintain hardness better than Ni-P when they are overaged. The banded structure that was depicted in Fig. 4.4 is seen to have disappeared in Fig. 4.9. A layer of an intermetallic phase, which formed as a result of interdiffusion of nickel and the steel substrate is alsoshown in Fig. 4.9. This layer develops upon heating above 600" C and thickens with increasing annealing time. While in this case adhesion was improved by interdiffusion, other substrates may form brittle intermetallic phases with nickel. Such layers could spa11 off and result in loss of adhesion. Fig. 4.7-Effects of aglng temperature and time on hardness for a Ni-P deposlt (11). T h a P r n n a r t i a nl f laetrnlass Nickel Fig. 4.8-Ellects 117 of aging temperature and time on hardness lor a Ni-B deposit (13). Fig. 4.9-Optical micrograph of cross-section of overaged Ni-P deposit on steel. NI,P grains ana an intermetalllc compound layer are evident. The banded structure that was seen in Fig. 4.4 has disappeared. 118 ELECTROLESS PLATING MECHANICAL PROPERTIES OF ELECTROLESS NICKEL The mechanical properties of electroless nickel plated in acidic solutions as a function of phosphorus content are listed in Table 4.1 (14). These properties weredetermined with a tensile-testing device described by Kim and Weil(l5). It is evident that electroless nickel is a relatively strong but brittle material. The low ductility is due to the microcrystalline and amorphous structures that essentially preclude plastic deformation (14). The deformation is therefore mostly elastic until fracture occurs. The modulus of elasticity appears to have a maximum in the intermediate composition range. A much lower value of 120 MPa of the modulus of elasticity was reported by other investigators (4,,11) for an alloy of 5 percent P. However, a9-percent P deposit had a modulus of 50 GPa (16), which is in the same range as the values in Table 4.1. Table 4.1 Mechanical Propertles of Nlckel-Phosphorus Deposits Composition, percent P 1t03 5 to 7 7 to 9 10 to 12 Modulus of elasticity GPa Msi 50-60 62-66 50-60 50-70 Tensile strength MPa Ksi 7.1-7.4 150-200 21-29 8.9-9.4 420-700 60-100 7.1-8.6 800-1100 114-157 650-900 93-129 7.1 Elongation, percent <1 <1 1 1 HKioo 650 580 550 500 It is evident from Table 4.1 that the tensile strength of the low-phosphorus, microcrystalline alloys is lower than that of the amorphous ones. Graham, Lindsay and Read (17) measured the mechanical properties of Ni-P deposits from alkaline solutions by bulge testing and found a sharp increase in the significant stress at fracture (which is essentially the same as the tensile strength) at about 7 percent P, where the transition from microcrystalline to amorphous occurs (6).The reported significant fracture stress values (17) of about 650to850 MPafor>7-percent Palloysagreefairly well with those listed in Table 4.1. Significant fracture stresses of 300 to 500 MPa were reported (17) for 5-percent-P deposits. Table 4.1 shows the ductility of electroless nickel as manifested by the elongation to be 1 percent or less over the whole range of compositions. All the deposits are therefore brittle in the as-plated condition. The Properties of Electroless Nickel 119 An increase in the tensile strength of Ni-P specimens plated on thin copper tubes, which were subsequently dissolved, from 450 MPa to 550 MPa has been observed (11) after heating to 200" C for 15 minutes. Heating to 750" C for 2 hours was found (17) to considerably increase the significant fracture stress for low-phosphorus deposits while that of the higher-phosphorus alloys decreased. Thus, the fracture stress of a 5-percent P deposit increased to about 800 MPa, while that of a 9-percent P alloy decreased to about 250 MPa. Hardness, the resistance of a material to permanent deformation by indentation, is an easily measured property, and therefore is most frequently determined by investigators of electroless nickel. It is useful in predicting abraske-wear properties but bears no direct relationship to the strength of a material (18). The hardness of as-plated Ni-P deposits falls in the range of 500to 600 kg/mm2as measured with a Knoop or Vickers indenter using a 100 g load. The Vickers numbers are generally greater than the Knoop hardnesses (18). There are a few special plating solutions that yield deposits of higher hardness. A gradual decrease in hardness with increasing phosphorus content has also been observed (19). As-plated Ni-6 deposits have a Knoop hardness number of about 700 (19). The composition appears not to have a great effect on the hardness of Ni-B deposits, which tend to be harder than Ni-P, especially after a long heat treatment. (See Fig. 4.8) Comparison of Figs. 4.1 and 4.2 shows that the eutectic temperature (where melting starts) is 1140" C for Ni-6 alloys, but only 880" C for Ni-P. As softening occurs at these temperatures, Ni-6 deposits possess a higher so-called hot hardness. The ability of electroless nickel to maintain its hardness at elevated temperatures is illustrated in Fig. 4.10 (20), which shows the hardness of Ni-P deposits measured at various temperatures. It is seen that hardness decreases linearly with increasing heat-treatment temperature up to 385" C. Above 385" C, the hardness decreases rapidly with increasing temperature and holding time. High-phosphorus deposits harden more slowly in the 260 to 300" C range, but also take longer to soften at 400 to 600" C than those with lower alloy contents. The slower decrease in the deposits with higher alloy contents is due to their containing a larger volume of the Ni,P phase. For example, under equilibrium conditions, which are essentially attained after prolonged heat treatment, the volume percentage of Ni3Pin an 8-percent P alloy is about 50 percent, and 100 percent in a 15-percent P deposit. A third element can also affect hardness. For instance, the addition of molybdenum increases the hardness of nickel-boron deposits (21). The hardness of Ni-Mo-P alloys heat treated at 400" C, where they also attain their maximum value, increases with increasing molybdenum content. The temperature at which Ni-Mo-B alloys reach their maximum hardness isafunction of composition. For example, an alloy containing 17 percent Mo and 0.3 percent B attains its maximum hardness of about 1000 HV when heat treated at 600" C. The adhesion between electroless nickel and non-metallic surfaces depends on an essentially mechanical bond. Deposition into micro-crevices results in a keying action. The preparation of the substrate surface therefore affects adhesion. The adhesive strength increases with increasing surface roughness 120 ELECTROLESS PLATING Flg. 4.10-Hot hardnessof electroless nlckel(20). 0 = 10.5 percent P, prlor heat treatment at 800' C for 1hr, A =8.0 peffiont P, 1hr at 600' C; B = 6.8 percent P, 1 hr at 600' C; 6.6 percent P, 1 hr at 6W0 C plus 1 hr at 750' C. o= (22).Adhesion to some metals can thus be enhanced by roughening their Surfaces. Such was found to be the case when electroless nickel was plated on aluminum alloys (23).Lossof adhesion has been attributed to a difference in the coefficients of thermal expansion of the deposit and substrate (24).It has already been pointed out that annealing above 600' C so as to form a diffusion layer can improve the bond between electroless nickel and steel. Annealing deposits on aluminum substrates at 150' C and those on steel at 200' C also improves adhesion. However, deposits on age-hardened aluminum should not be annealed above 130' C, in order to maintain the hardness of the substrate. The mechanical properties of parts can be adversely affected by coating them with electroless nickel. Metals such as high-strength steels, which are sensitive to hydrogen embrittlement, belong to this group. It is possible for sufficient hydrogen to be absorbed during electroless plating to cause failure in highstrength steels (25).Baking at about 200" C for several hours often relieves the hydrogen embrittlement. However, sometimes baking does not help, indicating that hydrogen is not the sole cause of poor mechanical properties in the substrate. Cracks that develop in the brittle electroless nickel coating during fatigue loading can propagate into the substrate and lower its endurance limit, Le., the largest stress at which it did not fail in fatigue loading after lo7cycles. For example, a low-carbon, high-strength steel originally had an endurance limit of 342 MPa, which was reduced to 260 MPa when the steel was coated with 25 pm of The Properties of Electroless Nickel 121 electroless nickel. Heat treatment at 400" C further reduced theendurance limit to 176 MPa. The reversal of the sign of the internal stress from compressive to tensile upon heat treating may have been the cause of the reduction in the endurance limit after annealing (19). Shot peening of parts prior to plating can improve the fatigue properties by putting the surface in a state of compression. INTERNAL STRESSES IN ELECTROLESS NICKEL DEPOSITS Internal stresses develop within deposits and are not due to externally applied forces. They can be classified as extrinsic and intrinsic. Extrinsic stresses are primarily due to differences in the thermal expansion coefficients of electroless nickel and the parts to be coated. As electroless nickel plating takes place at elevated solution temperatures, differences in shrinkage result when the coated parts are cooled to room temperature. If there is no loss of adhesion, tensile stresses develop in the component with the larger coefficient of thermal expansion, while the other one is in compression. Electroless nickel shrinks about 0.1 percent on cooling from 90° C (19). Depositson brassand aluminum, which have larger expansion coefficients than electroless nickel, are in a state of tensile stress. Deposits on beryllium and titanium, which have smaller coefficients, are in compression. The substrate surface is then in the opposite state of stress. Intrinsic stresses develop due to the deposition processes. In general, electroless nickel is not deposited initially as extended atom layers, but as discrete particles having the appearance of islands. The formation and subsequent joining of particles rather than lateral spreading of layers probably continues to be the growth mode as the deposit thickens. When these particles are pulled together by surface tension before the spaces between them are filled by plated metal, tensile stresses develop. Atom rearrangement can occur in a surface layer as it becomes covered during continuing deposition or during annealing, so as to change the interatomic distances. If the interatomic spacing decreases, the stresses are tensile. Compressive stresses can result when codeposited gases, such as hydrogen, diffuse into microvoids and expand them. If gases diffuse out of the deposit or into the substrate, tensile stresses develop in the deposit. The variations of the internal stress with phosphorus content of the electroless nickel plated on steel and aluminum are shown in Fig. 4.11 (26). A linear relationship between internal stress and the pH of the plating solution has also been found (27). At a pH of 4, where high-phosphorus deposits are produced, the stress was about -50 MPa, became tensile at a pH of 4.6, and reached a value of about 110 MPa when the pH was 6. On aluminum substrates, the stresses are generally compressive. A higher phosphorus content results in a lower tensile or a higher compressive stress. The values of the intrinsic plus extrinsic internal stresses shown in Fig. 4.1 1 are typical for electroless nickel. However, they can vary with the condition of the substrate and the instrumentation used for stress measurement. Chelating agents and additives to the plating solution can also change the intrinsic stresses significantly. 122 ELECTROLESS PLATING r "V'~"'V'U.7 "VII.C.I.) pZ.".F". Fig. 4.11-Eflects of phosphorus content on internal stress of Ni-P deposits plated on steel and aluminum substrates. Annealing increases tensile stresses and decreases compressive ones. Nickel-boron deposits generally exhibit higher tensile stresses than Ni-P alloys (28). Values of about 480 MPa have been measured for deposits containing 0.6 percent B. The tensile stresses decrease with increasing boron content to 310 MPa and 120 MPa for alloys of 1.3 percent Band 4.7 percent B, respectively (28). PHYSICAL PROPERTIES OF ELECTROLESS NICKEL The density of electroless nickel depends on the interatomic spacing and on the amount of porosity. The variation of the density with alloy contents is depicted in Fig. 4.12 (29). Data obtained at the National Bureau of Standards (30) are alSO shown. An essentially linear decrease with increasing phosphorus content is seen. As phosphorus atoms increasethe spacing between those of nickel atoms, the supersaturated solid solution has the lower density. The crystalline material is denser than the amorphous type (29,31). For example, a value of 7.9 g/cm' has been determined for amorphous electroless nickel containing 12 percent P, as compared to 8.1 g/cm' if it were crystalline (29). The interatomic spacing is also The Properfies of Electroless Nickel 123 Phosphorus or boron content, percent Fig. 4.12-Effecls of alloy composition on density for NI-P and Ni-B deposits (29). larger in the grain boundaries. As microcrystalline materials contain a considerable amount of grain boundary material, their density is lower than that of larger-grained electrodeposits. The density of nickel-boron deposits also varies essentially linearly with alloy content. Values of the electrical resistivity for electroless nickel alloys of various compositions are listed in Table 4.2. The electrical resistivity of electroless nickel is higher than that of electroplated nickel, which is about 8 pohm-cm (19), because alloying elements such as phosphorus and boron, especially when they are in solid solution, increase it. Also, as deviations from a regular crystal structure increase the electrical resistivity, amorphous deposits exhibit larger values than crystalline ones. Heat treatment, which results in the formation of intermetallic compounds and the crystallization of amorphous structures, substantially reduces the electrical resistivity. A sharp decrease in the resistivity in the temperature range where the amorphous structure crystallizes has been observed (33). The thermal conductivity is generally proportional to the electrical conductivity. It is thus possible to calculate the values of the thermal conductivity from the reciprocals of theelectrical resistivity. For high-phosphorus alloys, the 124 ELECTROLESS PLATING Table 4.2 Physical Properties of Electroless Nickel Density, Alloy g/cm3 1-3% P 0.1-2% B 5-7% P 4-5'10 6 0-9% P 5% 0 8.6 - >IO% P 0.3 0.5 0.1 0.3 <0 7% 0 7.0 Electrical resistivity, pohm-cm Coefficient of thermal expansion, pm/m/"K 30 5-13 50-70 - 70-90 90 <110 (19) 190 (26) 12 13 12 11 (32) 1 1 (13) thermal conductivity ranges from 0.01 to 0.02 cal/cm/sec/" K (34,35), compared to 0.2cal/cmfsec/" K for electroplated nickel. Values of the coefficient of thermal expansion are also listed in Table 4.2. It should be noted that on heating, when crystallization takes place and intermetallic phases form, volume changes occur that are reflected in the thermal expansion coefficient. A deposit containing 11 to 12 percent P had shrunk by 0.11 percent after heating to 300" C and cooling back to room temperature (36). Most of this shrinkage was due to structural changes. After a second heating and cooling cycle, the shrinkage was only 0.013 percent, indicating a more stable structure. The reported value of the thermal expansion coefficients for a 5 percent B deposit of 12 pm/m/"K decreased after heat treatment to 10.8 pmlm/"K (13). The magnetic properties of electroless NiP deposits depend on whether they are crystalline or amorphous. Crystalline deposits are ferromagnetic, while those having an amorphous structure are essentially non-magnetic (37). The amorphous, high-phosphorus alloys are often used under cobalt deposits on memory disks. The low-phosphorus, microcrystalline deposits have a relatively low coercivity, which is the external magnetic field that has to be applied for demagnetization. Values varying from 0 to 80 oersteds have been reported (19). The coercivity of electroplated nickel varies from 40 to 120 oersteds (19). The remnant flux density, which is proportional to the magnetization that remains when the outside field is removed, has reported values of about 400 to 600gauss, as compared to 2500 to 3300 gauss for nickel electroplated in a sulfamate solution. Most nickel-boron deposits are weakly ferromagnetic. The Properties of Electroless Nickel 125 After non-magnetic, electroless nickel deposits have been heat treated at 300 to 400" C, they are weakly ferromagnetic because of crystallization. The coercivities of the as-plated, microcrystalline deposits also increase when they are heat treated. A reason for the higher coercivities after heat treatment is that the paramagnetic intermetallic compound, Ni3P, impedes the movement of domain walls (6). The remnant flux density also increases after heat treatment to values ranging from 1000 to 3000 gauss (37). The Curie temperature, at which magnetism is lost on heating, decreases with increasing phosphorus content from 360" C for pure nickel, to 77' C when the alloy contains 7 percent P (38). Corrosion Resistance of Electroless Nickel Electroless nickel coatings are primarily used in engineering applications to provide protection for common metal surfaces exposed to corrosion as well as to wear. The corrosion protection is due to the low porosity of the coatings and the excellent resistance of nickel to many liquids and most atmospheric conditions. Electroless nickel prevents the contamination and discoloration of plasticizers, solvents, oils, glycols, monomers, and gases by metals such as iron, copper and aluminum. Significant savings in equipment costs are possible by replacing stainless steel with ordinary steel plated with electroless nickel. Stainless steel parts have been coated with electroless nickel to prevent pitting in the presence of chloride ions. The most important factors that determine the corrosion resistance of electroless nickel are: Substrate composition, structure and surface finish. Pretreatment of the substrate to achieve a clean, uniform surface. Adequate deposit thickness for the severity and time of exposure to corrosive conditions. The properties of the deposit (composition, porosity, internal stress) as determined by the pH, formulation and use (turnover) of the plating solution. Postplating treatments of the coating, such as passivation and annealing. The aggressiveness of the corrosive conditions. Generally, electroless nickel coatings have lower porosity and a more uniform thickness than the equivalent electroplated nickel and therefore provide better corrosion protection. In order for electroless nickel to be corrosion resistant, the pretreatment and plating conditions must achieve good adhesion and continuity of the coating. The integrity and corrosion resistance of thin coatings are generally evaluated by a neutral 5 percent salt spray test (ASTM 8117) and outdoor exposures. Electroless nickel coatings of about 9 percent P were found to provide longer protection than electroplated nickel. However, electroplated and electroless coatings containing 9 percent P behaved similarly (39). The difference in the electrochemical potential between electroless nickel and the substrate greatly affects what happens if there is a void or pore in the coating. The potential difference varies in different corrosive media, as seen in Table 4.3 (40). In an electrolytic cell, electroless nickel is the cathode against aluminum ELECTROLESS PLATING 126 and steel in most media, as indicated by the unbracketed numbers in Table4.3. If asmall areaof the substrate, which is the anode, is exposed, the current density, which is proportional to the corrosion rate, is very high there. A 300 mV difference will initiate and sustain corrosion of steel or aluminum substrates if the electroless nickel coating is not continuous. If the electroless nickel is the anode, as is the case for the bracketed numbers in Table 4.3, the coating corrodes sacrificially. However, as the anode area in this case is large, the current density and the corrosion rate are relatively low. Using the salt spray test, it was found (41) that periodic reverse alkaline cleaning prior to plating produced the most corrosion-resistant coating. If pickling is necessary, 10 percent sulfuric acid is preferable to hydrochloric acid. The pretreatment should be adequate to achieve a “clean”, film-free surface (42). Table 4.3 Potential Differences Between Electroless Nickel and Other Metals (40) Environment Aluminum Seawater Aerated tap water Deareated tap water 0.1N HCI 0.1 N HNOi 0.1N NaOH 3.5% CO?brine H2Sbrine 450 400 710 320 170 Potential difference, mV 304 stainless steel Mild steel 450 650 450 200 440 1160 [201 530 260 430 380 Outdoor exposure and salt spray tests have shown that electroless nickel coatings containing more than 9 percent phosphorus possess superior corrosion resistance to those with lower alloy contents. Compressively stressed deposits with higher phosphorus contents can be achieved by a pH less than 4.5 and the presence of strong chelating agents in the plating solution (43,44). One reason for the better corrosion resistance of coatings having higher phosphorus contents is that their more noble and passive polarization potential, which makes them less prone to pitting in such media as 3 percent NaCl and 10 percent HCI solutions (45). Another reason is that the amorphous microstructure is more homogeneous and there are no grain boundaries (46). The presence of a fibrous-appearing microstructure seen in the cross section of some electroless nickel deposits rendeis them more susceptible to corrosion, as evidenced in potentiodynamic and salt spray tests (47). The fibrous structure can result from sulfur-containing stabilizers, such as 2-mercaptobenzothiazole. T h e properties of Electroless Nickel 127 The banded structure shown in Fig. 4.4, which is a result of variations in the phosphorus content with thickness, can be beneficial (46) in that it can behave similarly to duplex nickel coatings. Coatings consisting of a sacrificial layer Of a lower phosphorus deposit over one of a higher alloy content can also behave similarly to duplex nickel (48). Tensile internal stresses render electroless nickel coatings more susceptible to corrosive attack. Internal stresses result in increased potential differences and, therefore, in lower breakdown potentials and higher corrosion currents (49). Such stresses can result from the deterioration of the plating solution due to the accumulation of orthophosphite and sulfate ions after several turnovers (50). It can be readily seen that differences in the composition, structure and properties can result in the large variations of from 24 to 1000 hours resistance observed in salt spray tests of thin (10 to 12 pm) electroless nickel coatings. The coating thickness also affects the corrosion resistance. On rough steel or aluminum surfaces, thicknesses of 50 to 75 pm are required for extended corrosion protection. Heat treatment in the temperature range of 300 to 400" C to achieve maximum hardness lowers the corrosion resistance of electroless nickel, probably as a result of microcracking. However, heat treatments at lower temperatures (in the 150 to 200' C range) have little effect on corrosion resistance. Improved corrosion resistance has been observed (51) after annealing at 600 to 700" C, because of improved bonding to steel substrates and improved integrity of the coating. Care must also be taken that heat treatment does not cause cracking of the coating as a result of shrinkage on metals with low thermal expansion coefficients, such as titanium and certain stainless steels. The salt spray resistance of most electroless nickel deposits can be improved significantly by passivation of the surface in a warm 1 percent chromic acid solution for 15 minutes. Considerable improvement in the results from the salt spray test after such a treatment was observed (52). Because of the many variables that affect the properties of electroless nickel coatings, it is difficult to predict their corrosion resistance. Electroless nickel should not be used in environments that attack unalloyed nickel. These environments include most organic and inorganic acids having a pH less than 4, as well as ammonium and halide salt solutions. Included also are solutions of chemical compounds that complex nickel. Electroless nickel has good resistance to alkaline solutions except ammonia and very concentrated (70 percent) hot caustic, which dissolves the phosphorus. Other liquids that attack nickel are carbonated and alcoholic beverages, coffee, fruit juices, vinegar, dextrose, bleach and fertilizers. Table 4.4 (53) shows laboratory corrosion rates of electroless nickel containing 8 to 9 percent Pin various liquids. Aeration of the liquids increased the corrosion rates, while heat treatment of the deposits at 750" C for 1 hour can improve resistance, probably because of the formation of passive surface layers (51). Field performance does not always correspond to observed laboratory test results. Therefore, Table 4.4 should be used cautiously. Service tests in the actual environment should be conducted if possible. There are many cases in 128 ELECTROLESS PLATING Table 4.4 Corrosion Resistance Tests of Electroless Nickel (9% Temp., Corrodant Acetaldehyde, waterfree Acetone Acrylonitrile Ammonium sulfide Amyl acetate Amyl chloride Beer Benzene Benzyl acetate Benzyl alcohol Calcium chloride, 48.5% Caprolactam monomer Caprylic acid Carbon disulfide Carbon tetrachloride Cresylic acid Detergent, 5% Ethyl alcohol Ethylene glycol Formaldehyde, 37% Gasoline Lactic acid, 80% Methyl alcohol Naptha Naphthenic acid Oleic acid Orange juice Perchloroethylene Petroleum (sour crude) Polyvinyl acetate Rosin size Sodium carbonate, 100/0 Sodium chloride, 3% Sodium hydroxide, 50% Sorbitol Stearic acid Sugar (liquid) Tall oil (crude) Toluol (nitration) Trichloroethylene Urea, 25 % solution Water, deionized Water, distilled O F 150 Room 150 120 Room Room 45 Room Room Room Room 185 150 Room Room 120 Room Room Room Room Room Room Room Room 150 max. Room Room 150 max. Room 150 max. 210 Room Room 250 150 max. 158 Room 150 150 max. 150 Room 180 Room Aeration Yes No Yes Yes No No No No No No No Yes Yes No No No No No Yes No No Yes No No Yes No No Yes No Yes Yes No No No Yes No No Yes Yes Yes Yes Yes No Heat Treated'. No No No No No No Yes No No No No No No No No No No No Yes Yes No Yes No No No No No No No No Yes No Yes No No No No No No No No No No P) Corroslon rate' MWyr fim/yr 0.02 0.003 0.016 0.15 0.0019 0.013 0.0078 0.0016 0.5 0.076 0.4 3.8"' 0.048 0.33 0.2 0.04 Zero Zero 0.0036 0.02 0.03 0.06 0.092 Zero Zero Zero Zero 0.01 0.037 0.0065 0.025 0.012 0.022 0.145 0.25 0.94 0.16 0.64 0.30 0.56 3.7"' Zero Zero Zero Zero 0.02 0.012 0.013 0.15 0.5 Zero 0.05 Zero Zero Zero 0.5 0.76 1.52 0.3 0.33 3.8"" 1.27 Zero Zero 0.04 1 .o Zero Zero 0.1 0.02 2.5"' Zero Zero 1 .o 0.04 0.023 0.5 0.58 Zero Zero 0.5 Zero Zero 0.029 0.74 0.02 'Corrosion rates are based on laboratorytests. Commodities listed in the table may vary from batch to batch in traceconstituentsthat couldaffect corrosion rates. Where large-scaleuse is contemplated.specificcorrosiondata should be obtained for the commodity in question. "Heat treated at 750" C for 1 hour. "'Not recommended. The Properties of Electroless Nickel 129 which electroless nickel has provided excellent protection from corrosion under many service conditions. Coatings containing 10 to 11 percent P have performed well on tools used in oil and gas wells when exposed to sour (carbon dioxide and hydrogen sulfide) gases (5435).Meat-cutting equipment has been protected by electroless nickel for many years. Electroless nickel has been substituted for stainless steel in some food packaging and processing applications, such as dough-mixing troughs, baking pans, electric grills, and wire baskets for deep frying. The Ni-8 alloys generally have poor salt spray and corrosion resistance, probably because they are porous and possess a fibrous structure. WEAR PROPERTIES OF ELECTROLESS NICKEL As was already pointed out, a primary reason for using electroless nickel is to protect substrates not only from corrosion, but also from wear. Wear is the gradual mechanical deterioration of contacting surfaces. One type, adhesive wear, results from the welding of the mating surfaces. As no actual surface is atomically smooth, it consists of asperities and depressions, Le., hills and valleys. When two surfaces are brought together, the area of contact consists primarily of the tops of the asperities, and is therefore only a small fraction of the total area. A relatively light load applied to the two mating parts thus results in a large stress, Le., the load divided by the contact area. The lateral movement of one surface relative to the other can remove any oxide or other soils on the tops of the asperities. Thus, the conditions for welding, namely intimate contact between two clean surfaces exist. Welding may be increased when the metals of the contacting surfaces are similar and mutually soluble in each other. The lateral movement can shear the welds again. If the shear fracture does not occur at the original weld, material from one surface adheres to the other. The resulting weight loss is adhesive wear. It is also possible that the shear fracture takes place on both sides of the original weld producing a separate particle. Then both surfaces undergo adhesive wear. Such particles, as well as ones from other sources can abrade the surfaces, causing a second type, namely abrasive wear. Abrasive wear can be minimized by making the surface harder and smoother. Hardening of a surface and lubrication reduce adhesive wear. If strong bonds develop under stress over a large portion of the contacting area, the mating surfaces may gall or seize, resulting in gross damage. Selecting dissimilar mating materials helps to avoid welding. Adhesive and abrasive wear are related, though no1directly, to the hardness of a surface, which is an indication of how much the tops of the asperities deform plastically. The greater the hardness, the less deformation, and consequently, there is less intimate contact and less welding and friction. Hard surfaces are also less likely to have the shear fracture occur at the original weld, resulting in less wear. Polishing the contacting surfaces also reduces wear because the contact area is larger and the stress that produces the intimate contact leading to welding is reduced. 130 ELECTROLESS PLATING Lubrication also reduces friction and wear by inhibiting the intimate contact. When hard particles, such as oxides, carbides, and diamonds are included in electroless nickel, they constitute the principal areas of contact. As these particles are less likely to weld, they reduce adhesive wear (18). However, if they are pulled out of the matrix they can cause abrasive wear. The inclusion of PTFE, which would tend to be smeared over the contacting surfaces, reduces friction by preventing the intimate contact that leads to welding and abrasion (56). The abrasive wear properties of electroless nickel can be improved by heat treatment. However, such heat treatment may lower its corrosion resistance. In general, thin electroless nickel coatings are only effective under relatively mild wear conditions. Severe or sudden loading should be avoided. Good adhesion to the substrate is essential for satisfactory wear performance. A hard coating on a soft substrate such as aluminum is easily disrupted and penetrated by a hard, rough contacting surface. Therefore, a hard substrate provides better support for electroless nickel coatings. Wear under working conditions is a very complex phenomenon. Among the many parameters that affect wear and make it difficult to control are surface hardness and finish; the microstructures and bulk properties of the mating materials; the contact area and shape; the type of motion, its velocity and duration; the temperature; the environment; the type of lubrication; and the coefficient of friction. The various laboratory tests can only provide indications of how parts will behave in service. Values of hardness and coefficients of friction can serve as a guide in selection of materials for a specific application. Trials under actual service conditions are still the only reliable indicatorsof how a part will wear. The coefficients of friction of electroless nickel in the as-plated condition are generally higher than those of electroplated chromium (19). Some values of the friction coefficient of a 9 percent P electroless nickel alloy against three different mating materials, with and without lubrication, are shown in Table 4.5 (19). The coefficients of friction of pins coated with Ni-P or Ni-B depositsare compared in Table 4.6 against various plates of different metals. Friction coefficients for lubricated Ni-B coated pins are also presented. It is evident that under dry conditions the Ni-B deposits have higher coefficients of friction, especially against copper and bronze. It can also be seen from Table 4.6 that the coefficients of friction do not bear a direct relationship to the hardness of the plates. The coefficient of friction for electroless nickel against steel appears to be relatively independent of phosphorus content. The least wear of electroless nickel against quenched steel is obtained when the deposit contains between 8 and 12 percent P after heat treatment at 400 to 600" C (57). Other wear test results are presented in Tables 4.7 and 4.8 (18). The wear data in Table 4.7 were obtained using a LFW-1 tester according to ASTM D2714-68. It compares the wear of a block against a rotating ring. The electroless nickel data in Table 4.8 were obtained with a Falex tester according to ASTM 02670-67. In this tester, a pin (journal) is rotated between two V-shaped blocks. The data in Tables 4.7 and 4.8 show a good correlation of hardness of the electroless nickel deposit to wear. The least wear resulted when the electroless nickel had been 131 The Properties of Electroless Nickel Table 4.5 Friction Coefficients of Several Mating Surfaces (19) Coefficientsof friction Unlubrlcated Lubricated Mating surfaces Electroless nickel (EN) vs. steel Cr vs. steel Steel vs. steel EN vs. EN Cr vs. Cr EN vs. Cr 0.38 0.19-0.23 galling 0.45 0.43 0.43 0.19-0.21 0.12-0.13 0.2 0.25 0.26 0.30 Table 4.6 Friction Coefficients of Electroless Nickel Against Different Metals (19) Metal Plate properties Hardness, Flnlsh, kg/mm2 Pm Steel' Steel" Gray iron Hard Cr Cu (plated) Bronze 'Hardened 105WCr6 steel "Normalized 105WCr6 steel. "'After surface v"s abraded. 960 310 210 960 105 200 2.6 3.0 2.9 1.2 2.7 1 .o Coefficients of plated pin vs. plate NI-P (11) Nl-B (13) dry dry lubricated 0.32 0.37 0.30 0.38 0.33 0.26 0.44 0.43 0.38 0.36 0.70"' 0.65 0.12 0.13 0.12 0.10 0.10 0.09 ELECTROLESS PLATING 132 Table 4.7 LFW-1 Wear Test Results Heat treatment "C hr Weight of loss, mg HVNlw friction mg HVNlW friction 523 743 1010 1060 0.09 0.09 0.11 0.1 1 102 585 724 988 1064 892 0.13 0.13 0.13 10 540 Coefficient of 1 1 1 EN-plated block vs. ring Coefficient Weight loss, As plated 260 260 400 EN-plated ring vs. block 50 13 1 not tested 0.10 0.10 9.0 8.8 2.8 2.3 1.7 'The hardness of the unplated steel block and ring were Ac 60and 65, respectively. In the tests of the plated ring vs. block, the load was 284 kg and the ring rotated for25.000 revolutions. In the plated block vs. ring test, the load was 68 kg and the ring rotated for 5000 revolutions. The lubricant was USP white oil. The rotational velocity of the ring was 72 rpm. Table 4.8 Falex Test Data of Rotating Pins vs. V Blocks (18)* EN deposit Heat treatment "C hr As plated 288 288 400 540 Chromium HV 590 2 880 16 1 1050 I 1100 750 1050 Unplated Pin W.L.' Plated block W.L. 0.2 0.1 0.1 0.2 0.1 1.9 6.6 1.2 1.2 0.5 0.4 0.5 Plated Pin W.L. Unpiated block W.L. 3.9 3.7 3.0 5.6 6.2 0.3 0.7 1.5 0.8 15.0 'The unplated V blocksand pins had hardnesses of RcPOto 24and60. respectively. The loads were94 kg applied for 1 hrand 182 kg applied for40 min. The pin rotated at a speed of 290 rpm. The lubricant was white oil. "Weight loss, rng. 133 The Promrfies of Electroless Nickel heat treated to HV 850 to 1100, as obtained at 260 to 290" C in 2 to 10 hours, or at 400" C in less than 1 hour. A minimum hardness of HV 850 is necessaryto obtain wear resistance comparable to that of hard chromium. The unlubricated wear rates of pins plated with electroless nickel containing 8.5 percent P against blocks of different metals determined in a testing device liketheone used toobtain thedatagiven inTable4.8areshown inTable4.9(58). Wear rates exceeding 10 mg/1000 cycles are considered to be unsatisfactory. It is thus seen that all the block materials, except chromium, which were tested against as-plated electroless nickel failed. Heat-treated, electroless nickel plated pins behave unsatisfactorily against chromium, stainless steel, and asplated electroless nickel. The wear rates of blocks of steel and thosecoated with electroless nickel heat treated at 400 and 600" C against electroless nickel pins heat treated at 400 and 600" C were satisfactory. It is apparent that electroless nickel should be used cautiously under unlubricated conditions. Table 4.9 Falex Unlubrlcated Wear Rates Of Electroless Nickel Coated Pins (58) Block material Steel Cr Stainless steel EN, as-plated EN, heated treated, 400" C EN, heat treated, 600" C Wear rates (wt. loss, mg/1000 cycles) AsHeat treated, Heat treated, 400' C 600" C plated 70 10 F' F 3 20 75 F 4 4 F 20 20 F 10 5 5 2 *Failureload-22.5 kg: rotation-290 rpm In unlubricated Falex wear tests on blocks with a hardness of Rc 20 to 24, Ni-B plated pins from an acidic (DMAB) solution performed poorly as compared to thosefrom a basic (sodium borohydride) solution, as well as Ni-P depositsfrom either acidic or alkaline sodium hypophosphite solutions. The data are shown in Table 4.10 (57).All deposits were heat treated for 1 hr at 400" C. The maximum load was 182 kg. Some Taber abrasion test data (16) are presented in Table 4.1 1 for chromium and electroless nickel alloys containing 10 percent P or 5 percent 6. The Taber Wear Index is the weight loss in mg per 1000 revolutions with a 1 kg load using resilient, abrasive (CS-10) wheels. ELECTROLESS PLATING 134 Table 4.10 Unlubricated Falex Wear and Hardness Data (59) Knoop hardness, Plated journal weight loss, Solution KNm mg Acid Ni-P Basic Ni-P Acid Ni-B Basic Ni-B 1088 990 1284 1195 64 16 419 68 Time to failure, min 6' 3' 7' 'Maximum load 182 g. Table 4.11 Taber Abrasion Data (16) Heat treatment Ni-P, as-plated Ni-P, 1 hr, 288" C Ni-P, 0.25-1 hr. 400" C Ni-P, 0.25-1 hr, 600" C Ni-8, as-plated Ni-B, 1 hr, 400" C Chromium Taber Wear Index* 15-20 10-15 6 4 8-12 4 2 'Taber wear index = mglweight IossI100 revs, CS-10 wheels, 1 kg load. The Properties of Elecfroless Nickel 135 It is apparent from Table 4.11 that the abrasion resistance increased with increasing heat treatment temperature. This improvement may be due to the larger grain size of the deposits. It is also apparent that Ni-B alloys are more abrasion resistant than Ni-P deposits. The best resistance to scoring (equal to that of chromium) was attained in Ni-P deposits heat treated for 2 hr at 289" C (60). In fretting wear tests it was found (61) that as-plated electroless nickel coatings containing 11 to 72 percent P on low alloy steel substrates behaved better than those heat treated to the maximum hardness. A minimum coating thickness of 25 pm (1 mil) was also found to be necessary. Duplex coatings consisting of 29-pm-thick hard Ni-P with 6 percent P deposited over a 40-pm-thick, somewhat more ductile layer of Ni-P with 12 percent P have protected hydraulic equipment subjected severe wear and corrosion conditions (62). The wear and abrasion applications of electroless nickel coatings can be summarized as follows: Coatings must be heat treated to a hardness greater than HV 800. Coating hardness on rotating partsshould be greater than that of the mating surface. Phosphorus content should be greater than 10 percent. Contacting surfaces should be smooth and lubricated. Electroless nickel coatings are not suitable for use under high shear and load conditions. REFERENCES 1. Binary Phase Diagrams, T.B. Massalski, chief ed., American Society for Metals, Metals Park, OH, 1986. 2. J.P. Randin and H.E. Hinterrnann, J. Electrochem. SOC.,115,480 (1968). 3. T. Omi, S. Kokunai and H. Yamamoto, Trans. Jpn. lnst. Metals, 17, 370 (1976). 4. W. Wiegand and K. Schwitzgebel, Metall, 21, 1024 (1967). 5. M. Sadeghi, P.D. Longfield and C.F. Beer, Trans. lnst. Metal finish.,61,141 (1983). 6. T. Yamasaki, H. lzumi and H. Sunada, Scripta Met., 15, 177 (1981). 7. E. Vafaei-Makhsoos, E.L. Thomas and L.E. Toth, Metall. Trans., 9A, 1449 (1978). 8. A.W. Goldenstein, W, Rostoker, F. Schlossberger and G. Gutzeit, J. Electrochem. SOC.,104, 104 (1957). 9. F. Ogburn and C.E. Johnson, Plating, 60, 1043 (1973). 10. C.C. Nee and R. Weil, Surface Tech., 25, 7 (1985). 136 ELECTROLESS PLATING 11. H. Wiegand, G. Heinke and K. Schwitzgebel, Metalloberflaeche, 22, 304 (1968). 12. W.G. Lee, Plating, 47 (1960). 13. H.G. Klein, H. Niederprum and E.M. Horn, Metalloberflaeche, 25, 305 (1971). 14. I . Kim, R. Weil and K. Parker, Plat. and Surf. Fin., 76(2), 62 (1989). 15. J. Kim and R. Weil, Testing of Metallic and Inorganic Coatings, ASTM STP 947, W.B. Harding and G. DiBari, eds., Am. SOC.Testing and Materials, Philadelphia, PA; p. 11-18. 16. K. Parker, unpublished data. 17. A.H. Graham, R.W. Lindsayand H.J. Read, J. Electrochem. SOC.,112,401 (1965). 18. K. Parker, Plating, 61, 834 (1974). 19. K. Parker i n The Properties of Electrodeposited Metals and Alloys, 2nd edition, W.H. Safranek,ed.; American ElectroplatersandSurface Finishers Society, Orlando, 1986; Chapter 23. 20. K.T. Ziehlke, “Hot Hardness of Electroless Nickel Coatings,” Union Carbide Nuclear Company Report K-1460 (1962). 21. G.O. Mallory, Plat. and Surf. fin., 63(6), 34 (1976). 22. N.F. Murphy and E.F. Swansey, Plating, 56,371 (1969). 23. S. Armyanov, T. Vanegelovaand R. Stoyanchev, Surf. Tech., 17,87 (1982). 24. T.N. Khoperia, Proc. Interfinish ’80, p. 147 (1980). 25. J.M:Hysak, “Current Solutions to Hydrogen Problems in Steels,” American SOC.for Metals, Metals Park, OH (1982); p. 84. 26. K. Parker and H. Shah, Plating, 58,230 (1971). 27. C. Baldwin and T.E. Such, Trans. Inst. Metal Finish., 46, 73 (1968). 28. G.O. Mallory, Plating, 58,319 (1971). 29. T. Schmidt et al., Nucl. Instr. and Methods, 199,359 (1982). 30. F. Ogburn, R.M. Schoonover and C.E. Johnson, Plat. and Surf. fin., 68(3), 45 (1981). 31. G.S. Cargill Ill, J. Appl. Phys., 41, 12 (1970). 32. G. Gutzeit, Trans. Inst. Metal finish., 33,383 (1956). 33. S.T. Pai, J.P. Morton and J.B. Brown, J. Appl. Phys., 43,282 (1972). 34. G. Gutzeit and E.T. Mapp, Corrosion Tech., 3,331 (1956). 35. A.A. Smith, Oak Ridge National Lab. Report Y2269 (1982). 36. M.W. Poore, Union Carbide Nucl. Div. Prelim. Report Y/DL-838 (1982). 37. M. Schwartz and G.O. Mallory, J. Electrochem. SOC.,123,606 (1976). 38. A.A. Albert et al., J. Appl. Phys., 38, 1258 (1967). 39. C.H. Minjer and A. Brenner, Plating, 44, 1297 (1957). 40. R.N. Duncan, Electroless Nickel Conference IV (1985). 41. K.B. Saubestre and J. Haydu, Proc. Surface 66, p. 192 (1966). 42. D.L. Snyder, Electroless Nickel Conference 111 (1983). 43. S. Yajima, Y. Togawa, S. Matsushita and T. Kanbe, Plat. and Surf. fin., 74(8), 66 (1987). 44. G.O. Mallory, Plating, 61, 1005 (1974). 45. M.L. Rothstein, Plat. andsurf. fin., 73(11), 44 (1986). The Properties of Electroless Nickel 137 46. M. Ratzker, D.S. Lashrnore and K.W. Pratt, ibid., 73(11),44 (1986). 47. G. Salvago et al., Proc. Interfinish '80, p. 162 (1980). 48. L.L.Gruss and F. Pearlstein, Plat. and Surf. Fin., 70(2),47 (1983). 49. G.O.Mallory, SAE Technical Paper 830693 (1983). 50. G.Linka and W. Riedel, Galvanotechnik, 77, 586 (1986). 51. K. Parker, Plat. andsurf. Fin., 68(12),71 (1981). 52. U.S. patent 3,088,846(1986). 53. J.R. Spraul, Plating, 46,1364 (1959). 54. J.F. Colaruotulo, B.V. Tilak and R.S. Jasinski, Electroless Nickel Conference IV (1985). 55. R.N. Duncan, Electroless Nickel Conference I1 (1982). 56. S.S. Tulsi, Trans. Inst. Metal Finish., 64,129 (1986). 57. J.P Randin and H.E. Hinterrnann, Trans. Inst. Metal Finishing, 72(9),53 (1974). 58. U. Ma and D.T. Gawne, Trans. Inst. Metal Finish., 64, 129 (1986). 59. R.F. Wrightrnan and F. Pearlstein, Metal Finishing, 72(9),53 (1974). 60. D. Butschkow and G. Gawrilov, Metalloberflaeche, 34, 238 (1980). 61. A.J. Gould, P.J. Boden and S.J. Harris, ibid., 61,97 (1983). 62. E. Schrneling and G. Schmidt, Electroless Nickel Conference 111 (1983).